** **

### UNIVERSITA’ DEGLI STUDI DI PARMA

**DOTTORATO DI RICERCA IN **
**INGEGNERIA CIVILE E ARCHITETTURA**

CICLO XXXIII

**ADVANCED METHODOLOGY **

**FOR FRETTING FATIGUE ASSESSMENT ** **OF METALLIC STRUCTURAL COMPONENTS **

Coordinatore:

Prof. Sandro Longo

Supervisor:

Prof.ssa Sabrina Vantadori

Co-supervisor:

Prof. Andrea Carpinteri

Candidato:

Andrea Zanichelli

Anni Accademici 2017/2018 - 2019/2020

**ABSTRACT**

*The present Ph.D. Thesis deals with the analysis of metallic structural *
*components subject to fretting fatigue in partial slip regime. An analytical *
*methodology for fretting fatigue assessment of structural components is proposed. *

*Such a methodology allows to evaluate both the initial crack path and the lifetime *
*of metallic structures under fretting fatigue elastic partial slip loading conditions *
*in high-cycle fatigue. *

*The proposed methodology consists in the joint application of the multiaxial *
*fatigue criterion by Carpinteri et al. together with the non-local approach (named *
*Critical Direction Method) by Araújo et al. The philosophy related to the theory of *
*the Critical Distance by Taylor is also taken into account in the procedure. *

*The stress field induced into two bodies in contact subject to fretting fatigue is *
*analysed in Chapter 2, since it represents an input data for the methodology. *

*Firstly, the damage process associated with fretting is described, by even *
*exploiting the concept of fretting map. Subsequently, the main methodologies *
*available in the literature to analyse fretting fatigue problems are briefly reviewed. *

*Finally, the analytical formulation implemented in the proposed methodology is *
*detailed. *

*Chapter 3 is devoted to the description of the advanced analytical methodology *
*proposed in the present Ph.D. Thesis for fretting fatigue assessment of structural *
*components. In particular, both the Critical Direction Method by Araújo et al., the *
*theory of the Critical Distance by Taylor, and the Carpinteri et al. criterion for *
*fretting fatigue are described. Then, the steps of the advanced methodology *
*proposed in the present Ph.D. Thesis are detailed. *

*Chapter 4 deals with the validation of the proposed analytical methodology. In *
*more detail, ten different experimental campaigns available in the literature and *

*related to fretting fatigue tests in partial slip conditions are examined. Eight *
*different materials, that is, four aluminium alloys, one titanium alloy and three *
*steels, are analysed. The results obtained in terms of both crack path orientation *
*and fatigue life are described and compared to the experimental ones available in *
*the literature, for each experimental campaign examined. *

*Finally, conclusions are summarised in Chapter 5. *

**INDEX**

**ABSTRACT ** **I**

**1 OBJECT AND OBJECTIVES OF THE PH.D. THESIS ** **1**

1.1 Object of study 1

1.2 Objectives of the Ph.D. Thesis 2

1.3 References 4

**2 STRESS FIELD DUE TO FRETTING FATIGUE ** **5**

2.1 Introduction 5

2.2 Fretting phenomenon: basic concepts 6

2.3 Analytical and numerical methods for fretting fatigue 10 2.4 Analytical solution for fretting fatigue in partial slip regime:

cylindrical contact 15

2.4.1 Constant normal load in contact problems 16

2.4.2 Static tangential load in contact problems 25 2.4.3 Cyclic tangential load in contact problems 38

2.4.4 Cyclic bulk load in contact problems 42

2.5 References 50

**3 FORMULATION OF AN ADVANCED METHODOLOGY **

**FOR FRETTING FATIGUE ASSESSMENT ** **55**

3.1 Introduction 55

3.2 Critical Direction Method 56

3.3 Theory of the Critical Distance 59

3.4 Carpinteri et al. criterion 62

3.4.1 Step I: determination of the critical plane orientation 63

3.4.2 Step II: fatigue failure assessment 66

3.5 Advanced methodology: description 71

3.6 References 78

**4 VALIDATION OF THE ADVANCED METHODOLOGY ** **PROPOSED FOR FRETTING FATIGUE ASSESSMENT ** **83**

4.1 Introduction 83

4.2 Al 2024-T351 aluminium alloy 85

4.2.1 Experimental campaign 85

4.2.2 Results 87

4.3 Al 7050-T7451 aluminium alloy 89

4.3.1 Experimental campaign 1 90

4.3.2 Results 91

4.3.3 Experimental campaign 2 94

4.3.4 Results 95

4.4 Al 7075-T651 aluminium alloy 98

4.4.1 Experimental campaign 1 98

4.4.2 Results 101

4.4.3 Experimental campaign 2 104

4.4.4 Results 105

4.5 Al-4Cu aluminium alloy 107

4.2.1 Experimental campaign 108

4.5.2 Results 110

4.6 Ti-6Al-4V titanium alloy 112

4.6.1 Experimental campaign 112

4.6.2 Results 113

4.7 EN8 steel 115

4.7.1 Experimental campaign 115

4.7.2 Results 116

4.8 AISI 1034 steel 118

4.8.1 Experimental campaign 118

4.8.2 Results 119

4.9 35NCD16 steel 121

4.9.1 Experimental campaign 121

4.9.2 Results 122

4.10 References 125

**5 CONCLUSIONS ** **129**

**NOMENCLATURE ** **133**

**LIST OF PUBLICATIONS ** **139**

Papers in International Journals 139

Conference papers 142

**1 **

**OBJECT AND OBJECTIVES OF THE PH.D. THESIS**

**1.1 Object of study **

The present Ph.D. Thesis deals with the analysis of metallic structural components subject to fretting fatigue in partial slip regime.

Fretting is a contact phenomenon that occurs when a structural component is clamped against another mechanical part in presence of small oscillatory relative displacements. In such a condition, relative micro-displacements arise at the contact surface. Two different regimes can be distinguished on the basis of the magnitude of such relative displacements:

i) *Gross slip regime, with micro-displacements generally of the order of *
*20 300 m*÷ µ . In such a condition, characterised by global relative motion
between the components, the main damage phenomenon is the material
wear (Berthier, 1989);

ii) *Partial slip regime, when the relative micro-displacements are of the order *
of few microns, together with a magnitude of the load clamping the
components sufficiently high to prevent complete sliding between them. In
such a condition, the contact surface consists of an inner stick region, with
no relative displacements, and an outer micro-slip region, and the main
damage phenomenon is the nucleation of cracks at the contact surface due
to high stress gradient (Hurricks,1970).

Superficial debris formation due to material wear is a complex long-term issue.

However, such a damage phenomenon is less dangerous than the crack nucleation and subsequent propagation when components are subjected to remote fatigue loading (Waterhouse, 1992). Therefore, partial slip regime has been recognised as the most damaging condition.

As a matter of fact, a remote fatigue loading, acting at least on one of the components under contact, is able to promote the evolution of surface cracks, that

can lead to failure of the fatigued component itself. This situation is referred to as
*fretting fatigue, which is well-known to be different from plain fatigue, mainly due *
to the high stress level that characterises the region near the contact surface
(Szolwinski, 1997). Moreover, fretting fatigue is a complex phenomenon that
depends on more than 50 parameters (Collins, 1965), which can be narrowed down
into eight groups: relative slip amplitude, number of loading cycles, frequency of
cyclic loading, magnitude and distribution of the contact pressure, local stress state,
material and surface conditions, temperature, and environments surrounding the
component surfaces (Sunde, 2018).

Fretting fatigue has been recognised as the primary failure mode in many in- service engineering components in different fields of application. Railway transport, where cracks nucleating due to rolling fatigue issues may lead to failure and consequent derailment, both air and sea transport, where damages related to detachment of layers or components in riveted joints could happen, and automotive area, where failure can occur in wheel spindle, turbine blades hook systems with the hub, fasten of crankshaft with bearing, are worth noting. Moreover, fretting fatigue affects orthopaedic implants, metal ropes and cables, and many other applications in which bolted joints are subjected to small oscillatory relative displacements or vibrations.

Most failures due to fretting fatigue occur in high-cycle fatigue regime conditions, where a large portion up to 90% of total fatigue life is spent in crack nucleation, whereas only a small amount is related to crack propagation (Namjoshi, 2002). Therefore, a crack-nucleation approach is desirable to be applied in order to assess the fatigue behaviour of fretting-affected components.

In such a context, an accurate analysis of fatigue behaviour of structural components subject to fretting fatigue appears to be of fundamental importance.

**1.2 Objectives of the Ph.D. Thesis **

An analytical methodology for fretting fatigue assessment of structural components is proposed in the present Ph.D. Thesis. In more detail, such a methodology may be employed in order to evaluate both the initial crack path and the lifetime of metallic structures under fretting fatigue elastic partial slip loading conditions in

high-cycle fatigue. Consequently, being based on linear-elastic formulations, it could be easily applied to practical situations in the industrial field.

The proposed methodology falls in the category of stress-based critical-plane approach. In particular, the criterion by Carpinteri et al. (Carpinteri, 2011) for metallic structures under multiaxial constant amplitude fatigue loading in high- cycle fatigue regime, originally proposed for plain fatigue conditions, is here extended to the case of fretting fatigue. The Carpinteri et al. criterion is implemented in conjunction with the Critical Direction Method proposed by Araújo et al. (Araújo, 2017), and the philosophy related to the theory of the Critical Distance by Taylor (Taylor, 2007) is also taken into account in the procedure.

The stress field induced into two bodies in contact subject to fretting fatigue is
**analysed in Chapter 2, since it represents an input data for the methodology. **

Firstly, the damage process associated with fretting is described, by even exploiting the concept of fretting map. Subsequently, the main methodologies available in the literature to analyse fretting fatigue problems are briefly reviewed. Finally, the analytical formulation implemented in the proposed methodology is detailed.

**Chapter 3 is devoted to the description of the advanced analytical methodology **
proposed in the present Ph.D. Thesis for fretting fatigue assessment of structural
components. In particular, both the Critical Direction Method by Araújo et al., the
theory of the Critical Distance by Taylor, and the Carpinteri et al. criterion for
fretting fatigue are described. Then, the steps of the advanced methodology
proposed in the present Ph.D. Thesis are detailed.

**Chapter 4 deals with the validation of the proposed analytical methodology. In **
more detail, ten different experimental campaigns available in the literature and
related to fretting fatigue tests in partial slip conditions are examined. Eight
different materials, that is, four aluminium alloys, one titanium alloy and three
steels, are analysed. The results obtained in terms of both crack path orientation
and fatigue life are described and compared to the experimental ones available in
the literature, for each experimental campaign examined.

**Finally, conclusions are summarised in Chapter 5. **

**1.3 References**

Araújo J.A., Almeida G.M.J., Ferreira J.L.A., da Silva C.R.M., Castro F.C. Early
*cracking orientation under high stress gradients: The fretting case. International *
*Journal of Fatigue, 2017; 100: 611-618. *

*Berthier Y., Vincent L., Godet M. Fretting fatigue and fretting wear. Tribology *
*International, 1989; 22: 235-242. *

Carpinteri A., Spagnoli A., Vantadori S. Multiaxial fatigue assessment using a
*simplified critical plane-based criterion. International Journal of Fatigue, 2011; *

33: 969-976.

*Collins J.A. Fretting-fatigue damage-factor determination. Journal of Engineering *
*for Industry, 1965; 87, 3: 298-302. *

*Hurricks P.L. Mechanism of fretting. Wear, 1970; 15: 389-409. *

Namjoshi S.A., Mall S., Jain V.K., Jin O. Fretting fatigue crack initiation
*mechanism in Ti-6Al-4V. Fatigue and Fracture of Engineering Materials and *
*Structures, 2002; 25, 10: 955-964. *

Sunde S.L., Berto F., Haugen B. Predicting fretting fatigue in engineering design.

*International Journal of Fatigue, 2018; 117: 314-326. *

Szolwinski M.P., Farris T.N. Mechanics of fretting fatigue crack formation.

*International Journal of Fatigue, 1997; 19: 39-49. *

*Taylor D. The Theory of Critical Distances: A New Perspective in Fracture *
*Mechanics. UK: Elsevier; 2007. *

*Waterhouse R.B. The problems of fretting fatigue testing. In: Attia M.H., *
*Waterhouse R.B., editors. Standardization of fretting fatigue test methods and *
*equipment. ASTM STP 1159, Philadelphia, 1992, 13-19. *

**2 **

**STRESS FIELD DUE TO FRETTING FATIGUE**

**2.1 Introduction **

The present Chapter deals with the analysis of the stress field induced into two bodies in contact, subject to fretting fatigue.

Firstly, the damage process associated with fretting is described. Moreover, the loading conditions that characterise such a phenomenon, that are fretting wear and fretting fatigue, are analysed and the mechanical behaviour under such conditions is described by exploiting the concept of fretting map.

Subsequently, the main methodologies available in the literature to analyse fretting fatigue problems are briefly reviewed. Such methodologies are based on both analytical and numerical solutions.

The methodology proposed in the present Ph.D. Thesis belongs to the field of the stress-based critical plane approach. In particular, the multiaxial fatigue criterion proposed by Carpinteri et al. (Carpinteri, 2011) is used in conjunction with the Critical Direction method proposed by Araújo et al. (Araújo, 2017) and the theory of the Critical Distance by Taylor (Taylor, 2007).

Finally, the analytical formulation implemented in such a methodology is detailed in the case of cylindrical contact, because the advanced methodology proposed in the present Ph.D. Thesis is verified by taking into account experimental fretting fatigue tests in partial slip conditions. Although the application of the above methodology to simple cases, such as cylinder-to-flat fretting fatigue tests, may appear restrictive because of its simplicity, it is fundamental for understanding the phenomenon of fretting fatigue. Moreover, in order to study more complex geometries, numerical approaches based on finite element models would be more suitable. However, the calibration of such models is quite difficult, and analytical solutions (such as the one implemented in the

methodology proposed in the present Ph.D. Thesis) are often employed for calibration, in order to achieve more reliable results.

**2.2 Fretting phenomenon: basic concepts **

Many in-service engineering components are subjected to a large number of vibrations. When such components are clamped against a different mechanical part by means of a normal load, relative cyclic nano-/micro-displacements arise at contact surface. This contact phenomenon is named fretting (Nowell, 2005;

Waterhouse, 1992).

The damage process associated with fretting is caused by the synergistic contribution of wear, corrosion, and crack nucleation and growth (Waterhouse, 1972). According to Hurricks (Hurricks, 1970), a typical damage mechanism can be observed in engineering materials subject to fretting.

The scarring of the superficial oxide layer is the initial mechanism that can be observed (Sunde, 2018). Then, the formation of cold-welds at the surface asperities appears, thus modifying the friction between the contact surfaces. In particular, the value of the friction coefficient has experimentally been observed to increase during the first few hundreds of loading cycles (Hills, 1998).

When the above micro-welds break and wear off, micro-debris appear between the contact surfaces (Szolwinski, 1997). Although such debris may initially promote the abrasion phenomenon, they act as a protective layer (named third body) reducing the wear of the material (Berthier, 1989).

As the number of loading cycles increases, plastic deformations take place near the contact surface, thus resulting in possible nucleation of several grain-sized microcracks (Endo, 1976). When such microcracks affect the superficial oxide layer, additional microdebris arise. This mechanism, together with corrosive environmental conditions, accelerates the wear process.

In such a condition, if a cyclic loading is applied to one of the members of the contact, the propagation of one or more of the aforementioned microcracks into the bulk material is promoted. It should be highlighted that the near-surface crack nucleation stage is dominated by the high stress gradient due to contact and

strongly depends on the material microstructure, whereas remote fatigue loading mainly affects the crack propagation stage (Nowell, 1990).

As far as the loading conditions are concerned, fretting wear and fretting fatigue can be distinguished (Waterhouse, 1992). Fretting wear loading condition is attained when at least one of the members of the contact is subjected to an external cyclic motion, whereas fretting fatigue loading condition is attained when at least one of the members of the contact is subjected to an external cyclic load.

In both such conditions either partial slip or gross slip regime may occur.

According to the theoretical model by Mindlin (Mindlin, 1949), partial slip regime is attained when the tangential force remains lower than the product of the normal load and the static coefficient of friction, and there are parts of contact where no slip occurs. The fretting loop in a tangential force-displacement plane is elliptical (Hannel, 2001). On the other hand, gross slip regime is attained when the tangential force is equal to the above product, and slip occurs across the whole contact. The fretting loop is trapezoidal (Hannel, 2001).

In order to properly describe the mechanical behaviour under both fretting wear and fretting fatigue, the concept of fretting map can be exploited. Such a tool is a visual description of the fretting phenomenon, built in order to characterise the fretting problem and distinguish the regimes involved. In particular, by means of fretting maps, it is possible to distinguish the regime of fretting contact in terms of:

i) Relative displacements, thus identifying stick (that is, no sliding), mixed stick and slip, or gross slip;

ii) Surface degradation, thus identifying fatigue, wear, or oxidation attack;

iii) Fretting loop shape, thus identifying linear, elliptical or trapezoidal shape.

A review of the main fretting maps available in the literature is given by Zhou et al. (Zhou, 2006). The concept of fretting map under fretting wear loading condition was initially proposed by Vingsbo and Soderberg (Vingsbo, 1988). They identified the slip amplitude as the most significant parameter. Therefore, they built different fretting maps, where the normal force, the frequency of vibration, the fretting wear rate, or the fretting lifetime were generally identified as a function of the slip amplitude.

**Vingsbo and Soderberg experimentally identified three regimes (Figure 2.1): **

i) Stick regime, characterised by no sliding at the interface and very limited wear and oxidation in correspondence of individual asperities. The fretting loop collapses in a segment;

ii) Mixed stick-slip regime, characterized by a central stick area and a surrounding annular slip area. Extensive crack formation (fatigue) arises in the slip area with release of particles from cracks (wear), and wear and oxidation appear at the shear fractured individual asperities in the stick area. The fretting loop has an elliptical shape;

iii) Gross slip regime, characterized by slip that takes place across the whole contact area, extensive wear with sliding marks in fretting direction and material delamination and detach of particles, and oxidation with detach of oxide flakes. Wear and oxidation are strongly coupled in such a regime.

The fretting loop has a trapezoidal shape.

**Figure 2.1 Example of fretting map under fretting wear loading condition proposed ***by Vingsbo and Soderberg (Vingsbo, 1988).*

Subsequently, Zhou et al. (Zhou, 1990; Zhou, 1992; Zhou, 1995) proposed the
*running condition fretting map (RCFM), where the fretting regimes are *
distinguished in partial slip regime, mixed fretting regime and gross slip regime,

depending on both displacement amplitude and number of loading cycles. More precisely, the regimes experimentally identified are (Figure 2.2a):

i) Partial slip regime, attained for small displacement amplitude values where, during the entire test, the contact behaves as in partial slip regime described by Mindlin or, in an equivalent way, in the mixed stick-slip regime described by Vingsbo and Soderberg. The fretting loop has an elliptical shape during the whole test;

ii) Mixed fretting regime, attained for intermediate displacement amplitude values, associated with an unstable fretting loop, that may have a trapezoidal shape or an elliptical shape depending on the number of loading cycles. The Mindlin model is not valid in such a regime;

iii) Gross slip regime, attained for large displacement amplitude values where, during the whole test, the contact behaves as in the gross slip regime described by both Mindlin and Vingsbo and Soderberg. The fretting loop has a trapezoidal shape during the whole test.

**Figure 2.2 (a) Running condition fretting map and (b) material response fretting map.**

Note that Zhou et al. ignored the stick regime highlighted by Vingsbo and Soderberg suggesting, in agreement with Mindlin, that there are always some regions of the contact experiencing slip and, therefore, no stick regime can actually exist.

Moreover, the regime definitions by Zhou et al. are more realistic than those
previously presented, because both Mindlin and Vingsbo and Soderberg neglected
the early stage of fretting process (that is, what happens below 10^{4} loading cycles)
and therefore were not able to capture the mixed fretting regime.

*Another fretting map, named material response fretting map *(MRFM), was
proposed by Heredia and Fouvry (Heredia, 2010). In such a fretting map, no
damage domain, cracking domain, competition domain, and wear domain are
**distinguished (Figure 2.2b). **

**Concerning the correspondence between RCFM and MRFM shown in Figure *** 2.2, partial slip regime is divided into a security domain, without damage, and a *
domain where cracking appears. On the other hand, gross slip regime is associated
with wear and oxidation, whereas mixed fretting regime generates competition
between cracking and wear.

Both fretting wear and fretting fatigue conditions have been widely investigated in last decades. In particular, fretting fatigue has been recognised as a primary failure mode across a wide range of structural components. Therefore, the main analytical and numerical solutions available in the literature for the case of fretting fatigue are reviewed in the following Section.

**2.3 Analytical and numerical methods for fretting fatigue **

Fretting fatigue has been recognised as a primary failure mode across a wide range of structural components, such as dovetail joints, bolt and riveted joints, spline coupling, running cables, and overhead conductors (Araújo, 2016; Juoksukangas, 2016; Moraes, 2018; Ruiz, 1984). Such a phenomenon is well-known to differ from plain fatigue, especially because of the high stress-gradient near the surface of the component due to contact.

The analytical studies of contact date back to the end of XIX century, when Hertz (Hertz, 1882) studied frictionless contact between linear elastic spherical

half-spaces. The Hertzian solution was then extended by many researchers, in order to find closed form solutions for different cases. Johnson et al. (Johnson, 1971) included the adhesive forces between the contact bodies, whereas Cattaneo (Cattaneo, 1938) and Mindlin (Mindlin, 1949) independently considered partial slips due to the presence of tangential loads. The Cattaneo-Mindlin case was then integrated by Nowell and Hills (Nowell, 1987) by taking into account the effect of a bulk cyclic stress on the stress components. Moreover, the Cattaneo-Mindlin problem was extended by Jager (Jager, 1998) to more general geometries and, subsequently, by Davies et al. (Davies, 2012) to varying normal loads.

Asymptotic analysis has also been employed to study the stress concentration in fretting fatigue, due to the analogy with cracks in fracture mechanics. Such a theory has been applied especially in complete contact problems with sharp contact edges, where the Hertzian theory fails. Williams (Williams, 1952) and Bogy (Bogy, 1968) proposed to evaluate the stress components as functions of the wedge angle, in elastically similar bodies and elastically dissimilar bodies, respectively.

The asymptotic theory has been applied also to incomplete contact in partial slip by Dini and Hills (Dini, 2004), who compared the results obtained with those deduced by using the Cattaneo-Mindlin solution, and by Fleury et al. (Fleury, 2017) who extended the analysis to more complex loading histories.

Analytical models are widely used for comparisons with experimental results and parametric studies. Moreover, such methods can be used to evaluate the stress field in real components, once the parameters involved have been adjusted.

On the other hand, numerical methods such as finite element methods, are becoming increasingly used, allowing to examine more complex geometries, loading histories, and external conditions. In general, when half-plane theory is violated, numerical methods are needed.

Finite element methods are available in the literature in order to take into account the effect of either wear or plasticity in the fretting fatigue modelling (Gandiolle, 2013; Madge, 2007). Moreover, microstructural effects, such as the damage evolution and the crack initiation, may be studied by including continuum damage mechanics in the finite element code (Zhang, 2012).

The extended finite element methods have recently attracted the interest of many researchers due to the possibility to enrich the solution of standard finite

element methods. In more detail, discontinuous functions can be implemented, thus providing the possibility to capture local and discontinuous effects. Moës et al. (Moës, 1999) proposed a model able to simulate the crack growth without the need for remeshing, and Giner et al. (Giner, 2008) were able to find good estimations in terms of stress intensity factors with a relatively coarse mesh by using singular expressions for complete contact as enrichment functions in the formulation of finite elements.

Nowadays, different approaches implementing either analytical or numerical models have been applied to assess the fatigue life of fretting affected components.

Some of those approaches consider both crack nucleation and crack propagation phase. Araújo and Nowell (Araújo, 2009) proposed a total life methodology for the evaluation of mixed low-high cycle fatigue tests. According to such a methodology, the number of cycles needed to nucleate a crack of a given length is added to the number of cycles for propagation. It is worth noting that the choice of the initiation crack length is arbitrary and may lead to very different results.

Navarro et al. (Navarro, 2003) proposed to define the initiation crack length by computing, in different material points along the crack path, the driving force for both initiation and propagation by using the Basquin equation and the Linear Elastic Fracture Mechanics (LEFM), respectively. The minimum depth at which the LEFM driving force was bigger than the one related to the initiation mechanism was assumed to be the initiation crack length. Consequently, the total life was obtained as the sum between the initiation number of cycles and the number of cycles for crack propagation until failure.

Some approaches related only to the crack propagation phase are available in the literature. Such approaches, based on the linear elastic fracture mechanics, aim to determine whether a crack will arrest after initiation by means of threshold curves for the stress intensity factors. By using a numerical methodology based on a stress-intensity factor criterion, Said et al. (Said, 2020) showed that cracks propagated up to a certain extent even in fully compressive state, and proposed a Mode II threshold. Moreover, Giannakopoulos et al. (Giannakopoulos, 1998) compared the contact stress with the stress singularities due to cracks. The crack growth in fretting fatigue was compared to a branching crack starting from a principal crack represented by the contact interface. The fretting fatigue life was

evaluated by means of the classical Paris law, by exploiting the asymptotic field description and inferring the order of singularity to be square-root bounded.

Nevertheless, damage models concerning the crack nucleation phase are mainly employed in fretting fatigue assessment, since crack nucleation life has been observed to be around 90% of the total fretting fatigue life (Walvekar, 2014). Such models may be classified according to Bhatti and Wahab (Bhatti, 2018) on the basis of the approach used to define failure. More precisely, four different approaches may be distinguished: fretting specific parameters (FSP) approach, continuum damage mechanics (CDM) approach, stress invariant (SI) approach, and critical plane (CP) approach.

In order to take into account the high frictional forces at the contact interface, fretting specific parameters incorporating the effect of slip amplitude have been proposed. The most widespread parameter was that proposed by Ruiz et al. (Ruiz, 1984), which combined relative slip amplitude with shear stress to obtain the frictional energy due to contact forces and later added tensile stress to such a frictional energy for better predicting the actual crack location. Such parameters provide a quantitative prediction of fretting fatigue behaviour, and are widely used in many industrial applications.

Continuum damage mechanics approach aims to describe the nucleation process inside a representative volume element at mesoscale, by employing mechanical variables. More precisely, a damage scalar variable incorporating the effect of mean stress, stress amplitude, loading history, material, and loading conditions is adopted. Different CDM models are available in the literature, such as those proposed by Bhattacharya and Ellingwood (Bhattacharya, 1998), Chaboche and Lesne (Chaboche, 1988) and Lemaitre (Lemaitre, 1985), in which the crack nucleation is assumed to occur when a critical value of damage is achieved. Since damage is computed as a scalar variable, no information can be obtained about crack orientation.

As far as the stress invariant approach is concerned, the parameter suggested by Crossland (Crossland, 1956) is worth noting. Such a parameter takes into account both the maximum amplitude of second invariant of the deviatoric stress tensor and the maximum hydrostatic pressure. This approach is characterised by a low time requesting computation, but it is not able to determine the crack orientation.

According to the critical plane approach, fatigue assessment is performed on a specific plane named critical plane, which is prone to be the crack nucleation plane.

This approach can further be classified as stress-based, strain-based, or strain- energy density based approach. Findley (Findley, 1959) and later McDiarmid (McDiarmid, 1991) proposed two different stress-based parameters for high-cycle fatigue regime, both of them depending on the maximum normal stress. Brown and Miller (Brown, 1973) suggested a strain-based evaluation of fatigue life, by proposing a linear combination of shear strain amplitude and maximum normal strain range. Fatemi and Socie (Fatemi, 1988) modified the Brown and Miller parameter by substituting the normal strain with the normal stress, in order to include the effect of non-proportional loading and mean stress. Moreover, among the strain energy density-based parameters, the one by Smith et al. (Smith, 1970), known as the Smith Watson and Topper (SWT) parameter (defined as maximum tensile stress multiplied by strain amplitude), and the one by Liu (Liu, 1993) (based on virtual strain energy) are the most widespread.

It is important to highlight that estimations can be improved by applying non- local approaches, that is, by taking into account either the stress state related to a material point at a certain distance from the contact zone or a mean stress state computed along a line or in a volume. Note that the strategy based on a mean state of stress was originally proposed for notched structural components: an analogy between notches and fretting fatigue seems to be appropriate since the notch effect in terms of stress concentration is similar to that due to the severe stress gradients in the contact zone for fretting fatigue (Araújo, 2016).

In the context of critical plane approach, Araújo et al. (Araújo, 2020) employed a finite element method that incorporated wear and a critical plane-based criterion coupled with a critical distance varying with fatigue life, in order to numerically analyse fretting fatigue tests on wires taken from overhead conductors. The approach showed reasonably accurate estimation of fretting fatigue life in medium- high cycle regime.

The methodology proposed in the present Ph.D. Thesis belongs to the field of stress-based critical plane approach. In particular, the multiaxial fatigue criterion proposed by Carpinteri et al. (Carpinteri, 2011) is implemented in conjunction with the Critical Direction method proposed by Araújo et al. (Araújo, 2017) and the

theory of the Critical Distance by Taylor (Taylor, 2007). The stress field used as input for the criterion is analytically evaluated by using the closed-form solution by Johnson (Johnson, 1985), based on the formalisms by Hertz (Hertz, 1896), Cattaneo (Cattaneo, 1938) and Mindlin (Mindlin, 1949), and McEwen (McEwen, 1949), together with the closed-form solution by Nowell and Hills (Nowell, 1987).

In more detail, such an analytical formulation in the case of cylindrical contact is discussed in the following Section, since the advanced methodology proposed in the present PhD Thesis is verified by taking into account experimental fretting fatigue tests in partial slip conditions.

**2.4 Analytical solution for fretting fatigue in partial slip regime: **

**cylindrical contact **

* Let us consider a typical fretting fatigue configuration (Figure 2.3), where two *
fretting pads, which may be characterised by either spherical or cylindrical shape,
are pushed against a dog-bone specimen in partial slip regime. The reference
frame,

*Oxyz*tangential force,

**, is shown in Figure 2.3. A normal constant force,**P , and a cyclic*Q t*( ), are applied to the pads, whereas the specimen experiences a cyclic axial stress, σ

*( )*

_{B}*t*, named bulk stress in the following, which is in-phase with

*Q t*( ).

*Q**(t)*

σ*B**(t)*
PAD

PAD

*O* *x*

*y* *z*

*Q**(t)*
*P*

*P*
SPECIMEN

**Figure 2.3 Typical cylinder-to-flat fretting fatigue test, in presence of both constant ***normal load, **P**, cyclic tangential load, *^{Q t}

### ( )

*, and cyclic bulk stress,*σ

*( )*

_{B}*t*

*.*

The stress field in the vicinity of the contact zone, in the case of fretting fatigue elastic partial slip loading condition, is detailed hereafter. Note that only the stress field in the case of cylindrical pads is presented in the following: nevertheless, the stress field in the case of spherical pads may be deduced in a similar way (Johnson, 1985).

**2.4.1 Constant normal load in contact problems **

Let us consider a contact problem with two non-conforming bodies, thus
characterized by different profiles. The contact zone between such solids consists
of a single point (or a line, depending on the bodies geometry), which coincides
with the origin of the reference frame *Oxyz in Figure 2.4. However, as far as an *
external load or displacement is applied, the two bodies deform and the contact
area becomes a finite area, whose sizes are a function of the magnitudes of applied
loads or displacements.

*O* *x*

*z* *y*

### body 2

### body 1

*z*

_{2}*z*

_{1}**Figure 2.4 Contact between non-conforming bodies, characterized by different general ***profiles.*

Therefore, a theory of contact is required to predict the shape and size of the contact surface, the magnitude and distribution of the surface tractions, and displacements and deformations induced within the two bodies.

In the region close to the contact zone, the surface profile of each body may be approximated by means of a parabolic shape, represented by the following quadratic expressions:

2 2

1 1 1 1

*z* = *A x* + *B y* + *C xy*

^{(2.1a)}2 2

2 2 2 2

*z* = *A x* + *B y* + *C xy*

^{(2.1b) }where higher order terms are neglected. *A , *_{1} *B , *_{1} *A , *_{2} *B are positive constants *_{2}
depending on the shape of solids brought into contact. It is possible to identify a
proper orientation of the *x and y axes (that is, x and *_{1} *y ) so that the term in xy *_{1}
*vanishes and Equations (2.1) become: *

2 2

1 1 1

1 1

1 1

2 ' 2 "

*z* *x* *y*

*R* *R*

= + *(2.2a)*

2 2

2 2 2

2 2

1 1

2 ' 2 "

*z* *x* *y*

*R* *R*

= − +

^{(2.2b) }

where *R , *_{1}' *R and *_{1}'' *R , *_{2}' *R*_{2}'' represent the surface radii of curvature for body 1
*and 2, respectively, in correspondence of the origin, O , of the reference frame. *

*Moreover, the distance, h , between the two surfaces may be written as follows: *

2 2 2 2

1 2

1 1

2 ' 2 "

*h* *z* *z* *x* *y* *Ax* *By*

*R* *R*

= + = + = + ^{(2.3)}

where *R and *' *R represent the main relative radii of curvature, whereas A and B *''
are positive constants. If the longitudinal axes of the two bodies are inclined to
each other by an angle α, it is possible to demonstrate that *A and B are defined *
by the following expressions:

1 1 2 2

1 1 1 1 1 1 1 1

2 ' " 2 ' " ' "

*A* *B*

*R* *R* *R* *R* *R* *R*

+ = + = + + +

^{(2.4a)}

2 2

1 1 2 2

1 1 2 2

1 1 1 1 1

2 ' " ' "

1 1 1 1

2 cos 2

' " ' "

*B* *A*

*R* *R* *R* *R*

*R* *R* *R* *R* α

− = − + − +

+ − −

*(2.4b) *

*By means of Equations 2.4, it can be deduced that: *

i) If the two bodies are solids of revolutions, then

1 2

1 1 1

*A* *B* 2

*R* *R*

+ = +

. The

*points characterised by the same value of h lay on a circle centred at the *
*origin O ; *

ii) If the two bodies are cylindrical and in contact along their longitudinal axes, then

1 2

1 1 1

*A* 2

*R* *R*

= +

and *B*=0. The points characterised by the
*same value of h lay on a straight line parallel to the longitudinal axis; *

iii) If the two bodies have general profiles, then *A and B are defined by *
general expressions. The points characterised by the same value of *h* lay
*on an ellipse centred at the origin O . *

We shall now consider the deformation (dotted line in * Figure 2.5) caused by *
the application of a normal load,

*P , on both bodies of general shape (chosen*convex for convenience).

Due to such a normal load, two points *T and *_{1} *T reasonably distant from the *_{2}
*contact surface move towards the origin of the reference system, O , whereas the *
points *S x y z and *_{1}( , , _{1}) *S*_{2}( , ,*x y z*_{2}) on the contact surface move along the *z axis *
by an amount equal to *u**z*1 and *u**z*2, measured from *T and *_{1} *T , respectively. In *_{2}
such a situation, the following two cases may arise:

*O* *x*

*z* *y*

*S*

_{2}*S*

_{1}### δ

_{2}

*P* *T*

_{2}*P*

### body 2

### body 1 *T*

_{1}*u*

_{z1}*u*

_{z2}### δ

_{1}

**Figure 2.5 Contact between non-conforming bodies, characterized by different general ***profiles: deformation due to constant normal load, **P* *(dashed lines).*

i) *S and *_{1} *S are coincident, that means that the two points are located within *_{2}
the contact region. In such a case, the following equality holds:

1 2 1 2

*z* *z*

*u* +*u* + = +*h* δ δ ^{(2.5)}

*And, by means of Equation (2.3), it becomes: *

2 2

1 2 1 2

*z* *z*

*u* +*u* = +δ δ −*Ax* −*By* ^{(2.6)}

ii) *S and *_{1} *S are not coincident, that means that the two points lie outside the *_{2}
contact region. In such a case, the following equality holds:

2 2

1 2 1 2

*z* *z*

*u* +*u* > +δ δ −*Ax* −*By* ^{(2.7)}

In order to analyse the deformation due to contact pressure, it is necessary to
determine the distribution of the pressure field at the contact interface, such that the
*resulting displacements, normal to the surfaces, satisfy both Equation (2.6) within *
*the contact area and Equation (2.7) outside such an area. *

Heinrich Hertz (Hertz, 1896) was the first one to achieve significant results
concerning the problem of the contact between two elastic bodies of general shape,
clamped against each other by means of a constant normal load. He considered
some hypotheses in order to simplify the problem. In more detail, by considering
the half-width *a* of the contact region, the radius *R of curvature of the two bodies, *
*the depth l of such bodies, the deformation *ε* _{y}* in correspondence of the yielding
of the material, the friction coefficient µ, Hertz assumed that:

1) *a*<<*R*, that is, the width of the contact surface is negligible with respect
to the radius of curvature for each body. Such a hypothesis allows us to
approximate the contact surfaces to an elastic half-space;

2) *a*<<*l*, that is, each body can be considered as an elastic half-space loaded
over an elliptical region at the surface. Such a hypothesis allows us to
obtain a stress/deformation field that is not influenced by the presence of
the solid boundary;

3) ε ε< * _{y}*, that is, the magnitude of the deformations near the contact region
allows us to apply the theory of elasticity;

4) µ =0, that is, the surfaces of the bodies are frictionless, that is, only normal stress is transferred.

Therefore, as far as two cylindrical bodies in contact along their longitudinal
*axes are considered, the contact surface consists in a strip of width 2a , lying *
* parallel to the axes of the cylinders (Figure 2.6). Such a contact surface may be *
considered as the limit of the elliptical surface that characterizes the contact
between general bodies, as one of the axes tends to infinite. It is important to
highlight that a plane strain condition may be assumed and, consequently, only

*x*

**and z coordinates are considered (Figure 2.6).***O*

*x*

*z*
*y*

**Figure 2.6 Contact between cylindrical bodies.**

*Equation (2.3) allows us to express the separation h between two cylindrical *
bodies as follows:

2 2

1 2

1 1 1 1

2 2

*h* *x* *x*

*R* *R* *R*

= + =

^{(2.8)}

being

1 2

1 1 1

*R* *R* *R*

= +

. Hence, for points lying on the contact surfaces, the
*condition represented by Equation (2.6) must be respected: *

1 2 1 2 2

1

*z* *z* 2

*u* *u* *x*

δ δ *R*

+ = + − ^{(2.9)}

whereas, for points outside the contact surface, the condition represented by
*Equation (2.7) holds: *

1 2 1 2 2

1

*z* *z* 2

*u* *u* *x*

δ δ *R*

+ > + − ^{(2.10)}

By means of the Hertzian theory, it is possible to uniquely determine the normal
pressure distribution, *p x , that satisfies Equations (2.9) and (2.10). More *( )
*precisely, by differentiating both contributions of Equation (2.9), it is possible to *
obtain:

1 2 1

*z* *z*

*u* *u*

*x* *x* *Rx*

∂ +∂ = −

∂ ∂ ^{(2.11)}

Moreover, by exploiting the results reported by Johnson (Johnson, 1985) related to the displacement field of a half-space due to the presence of a normal load, it is possible to write:

1 2 2 ( )

*

*a*

*z* *z*

*a*

*u* *u* *p s*

*x* *x* π*E* _{−} *x* *s* *ds*

∂ +∂ = −

∂ ∂

##

−

^{(2.12)}where *E represents the elastic modulus for plane strain condition. In the case of **
two bodies in contact, it becomes

2 2

1 2

1 2

1 1

1

*

*E* *E* *E*

ν ν

− −

= + .

*Therefore, by considering Equations (2.11) and (2.12), we can derive: *

( ) *

2

*a*

*a*

*p s* *E*

*ds* *x*

*x* *s* *R*

π

−

− =

##

^{(2.13)}from which the normal pressure distribution, ( )*p x , can be obtained: *

### (

^{2}

^{2}

### )

^{2}

^{2}

2 2

2 2

) * (

*x*
*a*

*P*
*x*

*a*
*x* *a*

*R*
*x* *E*

*p* + −

−

− −

= π π

π _{(2.14)}

In order to determine a distribution ( )*p x of compression on the whole contact *
region and a finite stress gradient at the edges of such an area, it is possible to
demonstrate (Hertz, 1896; Johnson, 1985) that the constant normal load *P must be *
equal to the following expression:

*R*
*E*
*P* *a*

4

2 *

=π ^{(2.15)}

*Therefore, by combining Equations (2.14) and (2.15), it is possible to determine *
the contact semi-width, *a*, between two cylindrical half spaces:

* 4

*E*
*R*
*a* *P*

= π ^{(2.16)}

Moreover, the normal pressure distribution arising at the contact interface
*between the two cylindrical bodies is obtained from Equation (2.14): *

2 2 2

) 2

( *a* *x*

*a*
*x* *P*

*p* = −

π ^{(2.17)}

*Such a distribution, named Hertzian contact pressure distribution, is *
* characterized by a parabolic shape (Figure 2.7) with a maximum value in the *
middle of the contact region (

*x*=0) equal to:

*O*

*x*

*z*
*y*

*P*

*a* *a*

body 2**p(x)**

*P*
body 1

**Figure 2.7 Contact pressure distribution, ( )***p x , at the interface of cylindrical bodies, *
*subject to constant normal load, **P**.*

*R*
*E*
*P*
*a*
*p* *P*

π π

* 2

0 = = *(2.18)*

The determination of stresses due to cylindrical contact was firstly provided in a
simplified form by McEwen (McEwen, 1949). In more detail, the components of
the stress tensor, produced by a general constant load *P in the vicinity of the *
contact zone, are given by:

2 2

0

2 2

1 2

*P*
*x*

*p* *z* *n*

*m* *z*

*a* *m* *n*

σ = − ^{} ^{} + ^{+} ^{}− ^{}
+

^{(2.19a)}

2 2

0

2 2

*P* 1

*z*

*p* *z* *n*

*a* *m* *m* *n*

σ = − ^{} − ^{+} ^{}

+ ^{(2.19b) }

2 2 0

2 2

2 2

0

2 2

for 0

for 0

*P*
*xz*

*p* *m* *z*

*n* *x*

*a* *m* *n*

*p* *m* *z*

*n* *x*

*a* *m* *n*

τ

− − ≥

+

=

−

<

+

*(2.19c) *

where the functions *m* and *n* are given by:

### ( )

^{2}

### ( )

2 1 2 2 2 2 2 2 2 2

2 4

*m* *a* *x* *z* *x z* *a* *x* *z*

= − + + + − + ^{(2.20a)}

### ( )

^{2}

### ( )

2 1 2 2 2 2 2 2 2 2

2 4

*n* = *a* −*x* +*z* + *x z* − *a* −*x* +*z* ^{(2.20b) }

Nevertheless, the influence of a cyclic tangential load on both stress and displacement fields is not taken into account by the Hertzian theory, and will be analysed in the following Section.

**2.4.2 Static tangential load in contact problems **

*The influence of a static tangential force, Q , on both stress and displacement fields *
within two bodies in contact is analysed in the present Section.

Let us consider two bodies of general profile, subject to both a normal load, *P , *
**and a tangential load, Q , as is shown in Figure 2.8. **

Firstly, the effect of the tangential force on size and shape of the contact
surfaces, as well as on the distribution of normal pressure on such an area, needs to
be analysed. In order to ensure the equilibrium, the distribution *q x y of *1

### ( )

, tangential load on surface 1 needs to be equal, but with opposite direction, to the distribution*q*2

### ( )

*x y of tangential load on surface 2:*,

### ( ) ( )

1 , 2 ,

*q* *x y* = −*q* *x y* *(2.21)*

*Q* *Q* *P*

*O* *x*

*z* *y*

*P* body 2

### body 1

**Figure 2.8 Contact between non-conforming bodies, characterized by different general ***profiles, subject to both constant normal load, **P**, and constant tangential load, **Q**.*

It is important to highlight that Boussinesq studies (Boussinesq, 1885) allow to
affirm that the normal displacement on contact surface is proportional, for each
body, to the value *G*1 2− ν *, where G represents the tangential elastic modulus. *

*Thus, by considering Equation (2.21), it can be written: *

### ( )

^{x}

^{y}

^{G}

^{u}### ( )

^{x}

^{y}*G* *u*

*z*

*z* ,

2 , 1

2

1 _{2} ^{2}

1 2

1

1

### ν

=− −### ν

− ^{(2.22)}

where ^{u}^{z}^{1}

### ( )

^{x y and }^{,}

^{u}

^{z}^{2}

### ( )

*x y represent the displacements of points lying on the*

^{,}contact surface of body 1 and body 2, respectively. The Poisson coefficients

*v*

_{1}

*and v and the tangential elastic moduli*

_{2}

*G and*

_{1}

*G are related to body 1 and body*

_{2}2, respectively.

*Equation (2.22) shows that, if the two bodies in contact are characterised by the *
same elastic properties, the tangential forces transmitted between them give rise to
normal displacements in body 1 that are equal to those in body 2, with opposite

direction. Therefore, the size and shape of the contact area is not affected by the
deformation of the surfaces. Consequently, such an area does not depend on the
*tangential load Q , and is function of the normal load P only. *

On the other hand, if the two bodies are characterised by different mechanical
properties, the normal pressure distribution, *p x , and the size and shape of the *( )
contact surface are influenced by the presence of the tangential load. Such an
influence was analysed by Bufler (Bufler, 1959), who analytically proved that the
presence of a tangential load causes both the shifting of centre and the increasing of
size of the contact surface. Nevertheless, such an influence is negligible for small
values of friction coefficient, typical of mechanical applications.

Therefore, in the following, the stresses and deformation due to the normal pressure are assumed to be independent of the stresses and deformation due to the tangential traction. In more detail, the superposition principle is used in order to define both stress and deformation fields.

As far as both a constant normal load, *P , and a constant tangential load, Q , are *
present, two cases may arise:

i) Total slip between the bodies, that is, the tangential force can be determined as a function of the normal load, by means of the friction coefficient

### µ

*=µ*

^{ ( Q}*);*

^{P}ii) Partial slip between the bodies, that is, even if no relative motions arise,
additional stresses due to friction are induced to the contact surface
*( Q*<µ*P*).

In the present Ph.D. Thesis, contact problems in partial slip conditions are analysed, due to the fact that total slip is rare in most of the structural components affected by contact problems (Hills, 1994). Moreover, as was highlighted by Madge et al. (Madge, 2007) and Araújo (Araújo, 2015), the most significant reduction of fatigue life occurs in partial slip regime.

Therefore, let us consider two bodies subject to a constant normal load, *P , and *
*a constant tangential load, Q , characterised by a partial slip regime, that is, *

*Q*<µ*P (Figure 2.9). *

*O* *x*

*z*
*y*

*T*_{1}*T*_{2}

### δ

*x1*

### δ

*x2*

*A*_{1}*A*_{2}*u*_{x1}

*u*_{x2}*P*

*P*
*Q*

*Q*
*T*_{1}*'*

*T*_{2}*'*
body 2

body 1

**Figure 2.9 Contact between non-conforming bodies, characterized by different general ***profiles: deformation due to both constant normal load, **P**, and constant tangential *

*load, **Q**.*

As far as partial slip regime is concerned, at least one point laying on the
contact surface is not affected by relative motion. More precisely, the contact
*region consists of two areas: the slip zone and the stick one. The first one is *
characterised by a relative slip between the contact surfaces, whereas the latter
presents a prefect adherence between the contact surfaces, without relative
motions.

Let us consider two points *T and *_{1} *T reasonably distant from the contact *_{2}
surface, with the corresponding displacements δ_{x}_{1}^{ and }δ_{x}_{2}, and two points *A *_{1}
and *A on the contact surface, with the corresponding displacements, *_{2} *u*_{x}_{1} and

2

*u**x* . The absolute displacement *s in the x direction between *_{x}*A and *_{1} *A may *_{2}
be expressed as follows:

### (

^{1}

### ) (

^{2}

### ) (

^{1}

^{2}

### ) ^{(} ^{)}

1 2 *x* 1 *x* 2 *x* *x* 1 2

*x* *x* *x* *x* *x* *x* *x*

*s* =*s* −*s* = *u* −δ − *u* −δ = *u* −*u* − δ −δ ^{(2.23)}

whereas the absolute displacement *s in the y direction may be expressed by: *_{y}

### (

^{1}

### ) (

^{2}

### ) (

^{1}

^{2}

### ) ( )

1 2 *y* 1 *y* 2 *y* *y* 1 2

*y* *y* *y* *y* *y* *y* *y*

*s* =*s* −*s* = *u* −δ − *u* −δ = *u* −*u* − δ −δ ^{(2.24)}

In the case of points *A and *_{1} *A located within the stick region, the absolute *_{2}
displacements *s and *_{x}*s are equal to zero and no relative motion arises. *_{y}*Consequently, Equations (2.23) and (2.24) become: *

1 2 1 2

*x* *x* *x* *x*

*u* −*u* =δ −δ ^{(2.25a)}

1 2 1 2

*y* *y* *y* *y*

*u* −*u* =δ −δ ^{(2.25b) }

It is possible to remark that all the points within the stick region undergo the
same displacement, regardless of the position of *A and *_{1} *A . Moreover, if the two *_{2}
bodies are characterised by the same value of elastic modulus, they are subjected to
*the same distribution of tangential load and thus, by considering Equation (2.21), it *
is possible to obtain:

1 2

*x* *x*

*u* = −*u* ^{(2.26a)}

1 2

*y* *y*

*u* = −*u* ^{(2.26b) }

Moreover, in order to assure that within the stick region no slip arises between
the bodies, the contact shear distribution, *q x y , must undergo the following *

### ( )

^{,}

condition: